- Nano Express
- Open Access
Free-Standing Sodium Titanate Ultralong Nanotube Membrane with Oil-Water Separation, Self-Cleaning, and Photocatalysis Properties
Nanoscale Research Letters volume 15, Article number: 22 (2020)
In this work, a free-standing sodium titanate ultralong nanotube membrane for multifunctional water purification has been prepared. For obtaining this free-standing membrane with good tenacity, one-dimensional (1D) sodium titanate ultralong nanotubes with a diameter of about 48 nm and length of hundreds of micrometers were prepared from TiO2 nanoparticles by a stirring hydrothermal method, which can be easily assembled into 2D membranes by facile vacuum filtration. After modified with methyltrimethoxysilane (MTMS), the free-standing membrane with hydrophobic surface possesses oil-water separation, self-cleaning and photocatalytic functions at the same time, which is favorable for the recovery of membrane and decontamination of various pollutants including oils, dust, and organic dyes from water. Furthermore, this membrane also exhibits excellent alkaline, acid, and corrosive salt resistance. This free-standing sodium titanate membrane with multifunction has potential applications in efficient wastewater purification and environmental remediation.
Oily water, arising from industrial sewage and frequent oil spill accidents, is harmful to the environment, animals, plants, and even humans and has aroused widespread concern throughout the world. The removal of intractable oil from water is a tough job [1, 2]. At present, many treatment methods for oily wastewater have been developed. Membrane separation technology has attracted much attention for its advantages of low energy consumption, flexibility, environmental friendliness, and high single-stage separation efficiency [3, 4]. Many researches have been carried out on improving the sustainability and efficiency of membrane separation technology. Szekely et al. noted that a large amount of wastewater generates during the fabrication process of the polymeric membrane, which makes membrane separation technology not as green as it is known. For making the membrane technology greener and more sustainable, they proposed a continuous wastewater treatment process to remove over 99% of the organic impurities by adsorbents and reuse these purified waters for the fabrication of membrane without detrimental effects on the performance of the final membrane . They also revealed the direct and indirect effects of the polarity of treatment solvent on membrane performance through systematical studies, which was successfully applied for improving the efficiency of pharmaceutical purification . More recently, many nano-engineering techniques were developed for the precise fabrication of porous membranes to meet specific separation required. Yang et al. prepared a solvent-free crystallization of MOF (ZIF-8) membranes by a layer-by-layer deposition process. The defect-free ZIF-8 membrane exhibited both higher H2 permeability and higher H2/CO2 selectivity simultaneously than the ever reported ZIF-8 membranes . Inspired by marine mussel, Szekely et al. for the first time fabricated a nanoengineered membrane formed by in situ polymerization of dopamine within a PBI support for the separation of polar aprotic solvents. The coating of PDA eliminated covalent cross-linking of the PBI backbone and achieved the highest permeance value of DMF . Manufacturing membranes with functional materials endow the membrane multifunction besides separation. Xu et al. reported a composite membrane composed of LiNbO3 coating layer and poly(ether sulfone) (PES) support. The presence of LiNbO3 endowed the membrane photocatalytic denitrification function . Multifunction membranes are aspired to effectively remove oil from various wastewaters [10,11,12].
Recently, more and more 1D inorganic materials were applied for obtaining free-standing membrane owing to their large specific surface area, low density, and high thermal conductivity and chemical sensitivity, as well as tunable metal and semiconductor properties [13,14,15,16]. 1D titanate materials not only have unique layered structure, good electrochemical, and optical properties but also possess excellent mechanical properties. These characteristics make it possible to be used in the fields of photocatalysis , adsorption [18, 19], sodium-ion battery , and energy storage . Recently, Wang et al. prepared a membrane for high-efficiency oil/water emulsion separation by using sodium titanate nanofibers, which were supported on a cellulose microfiber layer . In this work, a free-standing membrane was prepared by only using sodium titanate ultralong nanotubes with a length of hundreds of micrometers. This free-standing membrane exhibited excellent flexibility. After being modified with methyltrimethoxysilane (MTMS), the free-standing hydrophobic membrane possessed oil-water separation, self-cleaning, and photocatalysis functions, which are favorable for the recycling of separation membranes.
TiO2 powder (P25) was purchased from Deguassa Co. Ltd, Germany. Methyltrimethoxysilane (MTMS, ≥ 98%) and ethanol (CH3CH2OH, ≥ 95%) were purchased from Aladdin Reagent Company, China. Hydrochloric acid (HCl, 37%), sodium hydroxide (NaOH, ≥ 96%), and oxalic acid (≥ 99.5%) were obtained from Sinopharm Chemical Reagent Co. Ltd. All the chemical reagents were used in the experiment process without further purification. The deionized (DI) water was used throughout this experiment.
Synthesis of Na2Ti3O7 Ultralong Nanotubes
The synthesis of Na2Ti3O7 ultralong nanotubes was according to the literature procedure [22, 23]. Typically, 0.2 g of P25 powder was added to 30 mL of 10 M NaOH aqueous solution with continuous stirring for 5 min. Then the slurry was transferred into 50 mL Teflon-lined stainless-steel autoclave with a magnetic stirrer. The autoclave was put inside a silicon oil bath and the reaction temperature was set at 130 °C for 24 h. The stirring speed is 300 rpm. After the reaction, the autoclave was cooled to room temperature naturally. The precipitate was recovered and washed with distilled water several times to remove excess NaOH. The obtained product was further cleaned by using 0.1 M HCl solution three times to produce high purity Na2Ti3O7 ultralong nanotubes and washed again with distilled water for several times until pH = 7.
Synthesis of Free-Standing Na2Ti3O7 Porous Membrane and Surface Modification
Free-standing Na2Ti3O7 porous membrane was prepared by simple vacuum filtration without any other additives. Typically, Na2Ti3O7 ultralong nanotubes dispersing in ethanol with different concentrations were poured into the filter bottle and vacuum filtered for 10 min. The obtained membrane was dried in room temperature. By using different amounts of Na2Ti3O7 ultralong nanotubes, porous membranes with weights of 30 mg, 45 mg, 60 mg, and 75 mg were obtained, which are correspondingly defined as F-30, F-45, F-60, and F-75.
The obtained membranes were modified by dipping in MTMS sol-gel solution for 30 s and dried in room temperature for one night.
The morphology and size of the obtained samples were examined on a Tecnai G2 F30 S-Twin transmission electron microscope (TEM, FEI, USA) operated at 200 kV. The morphologies of the membranes were characterized by using a field emission scanning electron microscope (SEM, Hitachi S4800). Powder X-ray diffraction (XRD) patterns were recorded on a Bruker D8 Advance powder X-ray diffractometer at a scanning rate of 4° min−1, with Cu-Kα radiation (λ = 1.5406 Å) in the range of 10–60°. The contact angle (CA) of the membranes was measured on a Krüss DSA 30 (Krüss Company, Ltd., Germany) apparatus.
Results and Discussion
Na2Ti3O7 Ultralong Nanotubes and Free-Standing Membrane
Figure 1a is the XRD patterns of the product synthesized by stirring hydrothermal method. It can be seen that there are characteristic peaks at 11.1°, 18.8°, 25.4°, 30.3°, 34.8°, 36.7°, 39.2°, 44.2°, 48.9°, 50.2°, and 53.1°, which can be indexed as (100), (200), (011), (300), (− 303), (− 204), (− 401), (− 214), (020), (120) and (220) planes of Na2Ti3O7 (JCPDS, 59-0666), respectively [24, 25]. The basic building block of this kind of sodium titanate structure is TiO6 octahedron, the edge of which forms a negatively charged layered structure, and the opposite cation of Na+ is located between adjacent layers, resulting in a variable layer spacing [26,27,28]. XPS measurement further confirms the presence of Na, Ti, and O in the product with an atomic ratio of 1:1.58:4.04, which is in respect to the composition of Na2Ti3O7 (Additional file 1: Figure S1). Figure 1b shows the SEM image of the obtained Na2Ti3O7, which looks like ultralong “nanobelts”. It can be seen that the length of Na2Ti3O7 “nanobelts” can reach up to hundreds of micrometers with good flexibility, which will favor the formation of free-standing porous membranes. The ultralong “nanobelts” with excellent flexibility tend to array along the axis (Fig. 1c). However, high-resolution transmission electron microscope (HRTEM) image of a typical single “nanobelt” indicates that the “nanobelt” is actually a nanotubular structure (Fig. 1d). The lattice distance of 0.92 nm is corresponding to the interlayer spacing of (100) facet of layered Na2Ti3O7, suggesting the multiwall nanotubular structure of Na2Ti3O7.
In this study, the Na2Ti3O7 ultralong nanotubes were synthesized by hydrothermal method with stirring. Sun et al.  have systemically studied the formation mechanism of Na2Ti3O7 nanotubes in hydrothermal process without stirring. Generally, the length of Na2Ti3O7 nanotubes synthesized in the hydrothermal process without stirring is about 500 nm. These short nanotubes easily aggregate, which is not conducive to the formation of membranes (Fig. 2a). It has been reported that the length of titanate nanotubes can be controlled by a rotation speed during hydrothermal reaction [23, 30]. We found that the elongated Na2Ti3O7 nanotubes are easy to lay flat to form a film (Fig. 2b). But if using these Na2Ti3O7 nanotubes to form a free-standing membrane, polymer supports such as polyethylenimine (PEI) must be used . For obtaining a free-standing membrane without polymer supports, the amount of Na2Ti3O7 ultralong nanotubes was studied. SEM and TEM images in Fig. 3 indicate that the membranes consist of randomly oriented ultralong nanotubes and with the increase of membrane weight, Na2Ti3O7 ultralong nanotubes are denser. Figure 3a–f indicates that when the amount of Na2Ti3O7 ultralong nanotubes is small (30 mg and 45 mg), the assembly of Na2Ti3O7 ultralong nanotubes is loose and the adhesion between the nanotubes is insufficient. So, although these membranes have a certain tenacity but they tend to split into halves when they are bent (insets in Fig. 3c and f). But when the weight of membrane reaches up to 75 mg, this high content of nanotubes heavily intertwine, which leads to less freedom interspace between nanotubes and uneven of the membrane (Fig. 3j–l). Consequently, F-75 membrane with less tenacity is easily broken into small pieces (inset in Fig. 3l). F-60 membrane displays excellent tenacity due to its moderate nanotubes content, relative freedom between each other, and sufficient adhesion (Fig. 3g–i). So, F-60 was used for further studies. Additional file 1: Figure S2a–d indicates the corresponding thicknesses of F-30, F-45, F-60, and F-75 are 44 μm, 88 μm, 116 μm, and 210 μm, respectively (Table 1, Fig. 4). The thicknesses of these membranes have a linear relationship with the weight of Na2Ti3O7 ultralong nanotubes (Fig. 4). These results suggest that the thickness and tenacity of the membranes can be tuned through controlling the amount of Na2Ti3O7 ultralong nanotubes.
Wettability of the F-60 Membrane
Figure 5a indicates that both carbon tetrachloride (left side, stained by methyl red) and water (right side, stained by methylene blue) can spread and permeate the obtained F-60 membrane. The surface tension of carbon tetrachloride and water is 26.1 mN m−1 and 72.8 mN m−1 , respectively. In order to obtain a hydrophobic membrane for separating oil-water mixture, the surface tension of the F-60 membrane must be lower than ¼ of pure water (about 18 mN m−1) . Then the obtained F-60 membrane must be modified. In our study, the free-standing F-60 membrane is easily modified by dipping in MTMS sol due to its low surface energy and micro-nano rough structure [34,35,36]. The aging time of MTMS sol has an effect on the contact angle of the modified F-60 membrane. Figure 5b displays that with the increase of aging time, the contact angle of the modified F-60 membrane increase. But when the aging time is 14 h, the contact angle decreases. Because with the increase of aging time, MTMS gel with poor fluidity forms, which leads to the uneven surface of the F-60 membrane (Additional file 1: Figure S3) and the decrease of contact angle . The aging times range between 10 and 12 h are suitable for obtaining a hydrophobic membrane.
Multifunction of the Modified F-60 Membrane
Gravity driven oil/water separation has been achieved by many hydrophobic or hydrophilic membranes contained one-dimensional components [37,38,39,40]. Therefore, the modified F-60 membrane with hydrophobicity was firstly used for the separation of immiscible oil/water mixtures. The oil phase is carbon tetrachloride and the water phase is pure water, which are stained by methyl red and methylene blue, respectively. The oil/water separation process is carried out in a simple oil/water separating device as shown in Fig. 6a. The modified F-60 membrane was fixed between two glass tubes. When the oil/water mixture is poured onto the membrane, carbon tetrachloride permeated the membrane while water is kept in the upper side. Ten milliliters of carbon tetrachloride can pass through the membrane in 240 s. The calculated membrane flux is about 849 L m−2 h−1 and the separation efficiency for immiscible oil/water mixtures by the modified F-60 membrane reaches up to 99.7%. Generally, the water phase is not neutral especially for oily industrial wastewater. Figure 6b indicates that the modified F-60 membrane keeps high separation efficiency and even water phase contains corrosive acid, alkali, or salt.
Except for the different chemical contents in water, there is always dust or solid in industrial wastewater. Figure 7 indicates that the dust staying on the membrane after oil/water separation can be easily removed by water droplets due to the hydrophobic surfaces of the modified F-60 membrane.
The properties of materials contained in the membrane usually endow the membrane some special functions [41,42,43]. The membrane prepared using cross-linked cardanol-graphene oxide contains not only oil/water separation function but also a marked antibacterial activity that originates from the cardanol . Here, the specific surface areas and average pore diameter of the F-60 membrane are 240.4 m2 g−1 and 14.5 nm, respectively (Additional file 1: Figure S4). This porous structure and high specific surface area of the membrane may have a high adsorption capacity. Figure 7 indicates that after the oil/water separation process, the dye of methyl red in the oil phase can be partly adsorbed on the membrane. The self-cleaning process cannot clean the adsorbed dye. Taking advantage of photocatalytic property of sodium titanate [45,46,47], the adsorbed dye is expected to remove through photocatalysis reaction. Figure 8a–d displays that after 30 min irradiation with UV-light, almost all the adsorbed dye is removed. In order to demonstrate the removal of methyl red on the membrane due to photocatalysis reaction but not the decomposing of dye under UV-light irradiation, methyl red solution without photocatalyst was irradiated with UV-light. It can be seen from Fig. 8e that without photocatalyst, methyl red cannot be degraded by UV-light, which confirms the photocatalytic function of the sodium titanate membrane.
The MTMS modified F-60 membrane has light transmittance , so the Na2Ti3O7 nanotube can adsorb UV-light and generates electrons and holes. But the generation of hydroxyl radicals (Additional file 1: Figure S5) and the degradation of organic molecules need the medium of water. For investigating the mechanism of photocatalytic degradation of the organic molecule by MTMS modified F-60 membrane with superhydrophobic surface, a pure MTMS-modified F-60 membrane was irradiated under UV light for 30 min. It is found that after the irradiation of UV light, the contact angle of the membrane sharply decreased from 150.4° to less than 90° (Fig. 9a). This means that the surface property of MTMS-modified F-60 membrane changes. The FTIR result confirms that after UV light irradiation, Si–O–Si bonds in MTMS decrease, indicating these bonds are broken by UV light (Fig. 9b) [49,50,52]. The broken Si–O–Si will help the contact of water and light with Na2Ti3O7 nanotube and enhancing the photocatalytic performance. Furthermore, under the combined action of UV light and oxygen, MTMS is oxidized and more Si–OH bonds are observed in Fig. 9b; the reaction is shown in Eq. (1):
The broken Si–O–Si and oxidization of Si–CH3 by UV light make the generation of hydroxyl radicals and the degradation of organic molecular possible. When this membrane, after irradiation under UV light, was re-dipped in MTMS sol for a very short time, the contact angle of the membrane can rise back to 140° (Additional file 1: Figure S6). The recovery membrane can be reused for immiscible oil/water mixture separation and still preserve self-cleaning and photocatalysis functions. Currently, the membrane only can be recycled three times because the continuous increase of MTMS thickness results in a dramatic decrease of porosity of the membrane (Additional file 1: Figure S7). Studies are still ongoing for further improvement of the recovery rate of the membrane.
The above results indicate that the sodium titanate membrane preserves the multifunction of oil/water separation, self-cleaning, and photocatalysis simultaneously. Inorganic materials endow membranes multifunctional, which are required for treating industrial wastewater (Table 2).
In summary, we successfully prepared a multifunctional free-standing membrane with Na2Ti3O7 ultralong nanotubes. The diameter and the length of Na2Ti3O7 ultralong nanotubes are about 48 nm and hundreds of micrometers, respectively. The elongated Na2Ti3O7 ultralong nanotubes are easy to lay flat to form a membrane. The contact angle of the membrane can reach up to 150.4° after modifying by MTMS. The MTMS-modified free-standing membrane exhibits high membrane flux of 849 L m−2 h−1and separation efficiency of 99.7% for immiscible oil/water mixtures, even in strong alkaline, acid, or corrosive salt conditions. Additionally, the residual dust can be removed by self-cleaning function and adsorbed dyes on the membrane can be degraded in 30 min by photocatalytic function of the membrane. The free-standing sodium titanate membrane with a variety of functionalities of oil/water separation, self-cleaning, and photocatalysis will promise wide applications in environmental remediation and wastewater purification.
Availability of Data and Materials
The datasets used and/or analyzed during the current study are available from the corresponding author on reasonable request.
- F-30, F-45, F-60, and F-75:
Membranes with weights of 30 mg, 45 mg, 60 mg and 75 mg, respectively
High-resolution transmission electron microscope
Scanning electron microscope
Transmission electron microscope
Montgomery MA, Elimelech M (2007) Water and sanitation in developing countries: Including health in the equation. Environ Sci Technol 41:17–24
Oki T, Kanae S (2006) Global hydrological cycles and world water resources. Science 313:1068–1072
Shannon MA, Bohn PW, Elimelech M et al (2008) Science and technology for water purification in the coming decades. Nature 452:301–310
Kajitvichyanukul P, Hung Y-TH, Wang LK (2011) Membrane technologies for oil-water separation. In: Hung Y-T, Wang LK (eds) Handbook of Environmental Engineering, Vol 13: Membrane and desalination technologies. The Humana Press Inc., New York, pp 639–668
Razali M, Kim JF, Attfield M et al (2015) Sustainable wastewater treatment and recycling in membrane manufacturing. Green Chem 17:5196
Razali M, Didaskalou C, Kim JF et al (2017) Exploring and exploiting the effect of solvent treatment in membrane separations. ACS Appl Mater Interfaces 9:11279–11289
Yang P, Li Z, Gao Z et al (2019) Solvent-free crystallization of zeolitic imidazolate framework membrane via layer-by-layer deposition. ACS Sustainable Chem Eng 7:4158–4164
Zhao D, Kim JF, Ignacz G et al (2019) Bio-inspired robust membranes nanoengineered from interpenetrating polymer networks of polybenzimidazole/polydopamine. ACS Nano 13:125–133
Xu H, Li Y, Ding M et al (2018) Engineered photocatalytic material membrane assemblies for removing nitrate from water. ACS Sustainable Chem Eng 6:7042–7051
Wang YF, Lai CL, Wang XW et al (2016) Beads-on-string structured nanofibers for smart and reversible oil/water separation with outstanding antifouling property. ACS Appl Mater Interfaces 8:25612–25620
Yong J, Chen F, Huo J et al (2018) Green, biodegradable, underwater superoleophobic wood sheet for efficient oil/water separation. ACS omega 3:1395–1402
Wang B, Liang WX, Guo ZG et al (2015) Biomimetic super-lyophobic and super-lyophilic materials applied for oil/water separation: a new strategy beyond nature. Chem Soc Rev 44:336–361
Xiao Y, Huang J, Xu Y (2018) Hierarchical 1D nanofiber-2D nanosheet-shaped self-standing membranes for high-performance supercapacitors. J Mater Chem A 6:9161
Ge J, Fan G, Si Y et al (2016) Elastic and hierarchical porous carbon nanofibrous membranes incorporated with NiFe2O4 nanocrystals for high efficient capacitive energy storage. Nanoscale 8:2195–2204
Wang X, Dou L, Yang L et al (2017a) Hierarchical structured MnO2@SiO2 nanofibrous membranes with superb flexibility and enhanced catalytic performance. J Hazard Mater 324:203–212
Liu L, Liu Z, Bai H et al (2012) Concurrent filtration and solar photocatalytic disinfection/degradation using high-performance Ag/TiO2 nanofiber membrane. Water Res 46:1101–1112
Ide Y, Matsuoka M, Ogawa M (2010) Efficient visible-light-induced photocatalytic activity on gold-nanoparticle-supported layered titanate. J Am Chem Soc 132:16762–16764
Lopez-Munoz MJ, Arencibia A, Cerro L et al (2016) Adsorption of Hg(II) from aqueous solutions using TiO2 and titanate nanotube adsorbents. Appl Surf Sci 367:91–100
Yang D, Liu H, Zheng Z et al (2013) Titanate-based adsorbents for radioactive ions entrapment from water. Nanoscale 5:2232–2242
Fu SD, Ni JF, Xu Y et al (2016) Hydrogenation driven conductive Na2Ti3O7 nanoarrays as robust binder-free anodes for sodium-ion batteries. Nano Lett 16:4544–4551
Wang GY, Huang XY, Jiang PK (2017b) Bio-inspired fluoro-polydopamine meets barium titanate nanowires: a perfect combination to enhance energy storage capability of polymer nanocomposites. ACS Appl Mater Interfaces 9:7547–7555
Wang K, Yiming W, Saththasivam J et al (2017c) A flexible, robust and antifouling asymmetric membrane based on ultra-long ceramic/polymeric fibers for high-efficiency separation of oil/water emulsions. Nanoscale 9:9018–9025
Tang Y, Zhang Y, Deng J et al (2014a) Mechanical force-driven growth of elongated bending TiO2-based nanotubular materials for ultrafast rechargeable lithium ion batteries. Adv Mater 26:6111–6118
Sun M, Shen S, Wu Z et al (2018) Rice spike-like g-C3N4/TiO2 heterojunctions with tight-binding interface by using sodium titanate ultralong nanotube as precursor and template. Ceram Int 44(7):8125–8132
Bo A, Zhan H, Bell J et al (2014) Mechanical bending properties of sodium titanate (Na2Ti3O7) nanowires. RSC Adv 4:56970–56976
Dong WJ, Cogbill A, Zhang TR et al (2006) Multifunctional, catalytic nanowire membranes and the membrane-based 3D devices. J Phys Chem B 110:16819–16822
Sukpirom N, Lerner MM (2001) Preparation of organic-inorganic nanocomposites with a layered titanate. Chem Mater 13:2179–2185
Tang Y, Zhang Y, Deng J et al (2014b) Unravelling the correlation between the aspect ratio of nanotubular structures and their electrochemical performance to achieve high-rate and long-life lithium-ion batteries. Angew Chem Int Ed 53:13488–13492
Sun XM, Li YD (2003) Synthesis and characterization of ion-exchangeable titanate nanotubes. Chem Eur J 9:2229–2238
Torrente-Murciano L, Lapkin AA, Chadwick D (2010) Synthesis of high aspect ratio titanate nanotubes. J Mater Chem 20:6484–6489
Wen T, Zhao Z, Shen C et al (2016) Multifunctional flexible free-standing titanate nanobelt membranes as efficient sorbents for the removal of radioactive 90Sr2+ and 137Cs+ ions and oils. Scientific reports 6:20920
Deng D, Prendergast DP, MacFarlane J et al (2013) Hydrophobic meshes for oil spill recovery devices. ACS Appl Mater Interfaces 5:774–781
Meng HF, Wang ST, Xi JM et al (2008) Facile means of preparing superamphiphobic surfaces on common engineering metals. J Phys Chem C 112:11454–11458
Song JL, Rojas OJ (2013) Approaching super-hydrophobicity from cellulosic materials: a Review. Nord Pulp Pap Res J 28:216–238
Kota AK, Kwon G, Choi W et al (2012) Hygro-responsive membranes for effective oil-water separation. Nat Commun 3:1025
Mirvakili MN, Hatzikiriakos SG, Englezos P (2013) Superhydrophobic lignocellulosic wood fiber/mineral networks. ACS Appl Mater Interfaces 5:9057–9066
Sadeghi I, Govinna N, Cebe P et al (2019) Superoleophilic, mechanically strong electrospun membranes for fast and efficient gravity-driven oil/water separation. ACS Appl Polym Mater 1:765–776
Zhang YG, Zhu YJ, Xiong ZC et al (2018) Bioinspired ultralight inorganic aerogel for highly efficient air filtration and oil−water separation. ACS Appl Mater Interfaces 10:13019–13027
Li JJ, Zhou YN, Luo ZH (2015) Smart fiber membrane for pH-induced oil/water separation. ACS Appl. Mater. Interfaces 7:19643–19650
Huang M, Si Y, Tang X et al (2013) Gravity driven separation of emulsified oil-water mixtures utilizing in situ polymerized superhydrophobic and superoleophilic nanofibrous membranes. J Mater Chem A 1:14071
Gao SJ, Shi Z, Zhang WB (2014) Photoinduced superwetting single-walled carbon nanotube/TiO2 ultrathin network films for ultrafast separation of oil-in-water emulsions. ACS Nano 8:6344–6352
Si Y, Yan C, Hong F et al (2015) A general strategy for fabricating flexible magnetic silica nanofibrous membranes with multifunctionality. Chem Commun 51:12521
Zhu L, Gu L, Zhou Y et al (2011) Direct production of a free-standing titanate and titania nanofiber membrane with selective permeability and cleaning performance. J Mater Chem 21:12503–12510
Lim MY, Choi YS, Shin H et al (2018) Cross-linked graphene oxide membrane functionalized with self-cross-linkable and bactericidal cardanol for oil/water separation. ACS Appl Nano Mater 1:2600–2608
Chang YC, Lin JC, Wu SH (2018) One-step growth of Na2Ti3O7 nanorods for enhanced photocatalytic activities and recyclability. J Alloys Compd 749:955–960
Xu CY, Wu J, Zhang P et al (2013) Molten salt synthesis of Na2Ti3O7 and Na2Ti6O13 one-dimensional nanostructures and their photocatalytic and humidity sensing properties. CrystEngComm 15:3448–3454
Tsai CC, Chen LC, Yeh TF et al (2013) In situ Sn2+-incorporation synthesis of titanate nanotubes for photocatalytic dye degradation under visible light illumination. J Alloys Compd 546:95–101
Budunoglu H, Yildirim A, Guler MO et al (2011) Highly transparent, flexible, and thermally stable superhydrophobic ORMOSIL aerogel thin films. ACS Appl Mater Interfaces 3:539–545
Yang CS, Choi CK (2006) The characteristics of carbon-doped silicon oxide films with nano-pore structure deposited using UV-assisted PECVD. Thin Solid Films 506-507:8–12
Zakirov AS, Navamathavan R, Kang TW et al (2011) Effect of ultraviolet irradiation on the defect states and charge transport properties of low-k SiOC(-H) dielectric films deposited by UV-assisted PECVD. J Korean Phys Soc 58:71–72
Yang CS, Kannan M, Kyu CC (2005) Studies on the low dielectric SiOC(–H) thin films deposited using MTMS and oxygen as precursors by UV source assisted PECVD. Surf Coat Int 200:1624–1628
Chen RG, Zhang XG, Su ZH et al (2009) Perfectly hydrophobic silicone nanofiber coatings: preparation from methyltrialkoxysilanes and use as water-collecting substrate. J Phys Chem C 113:8350–8356
This work was supported by NSFC (51272157 and 51472160), Shanghai Nature Science Foundation (16ZR1423400, 18ZR1426400), and Science and Technology Commission of Shanghai Municipality (15JC1490700, 16JC1402200).
The authors declare that they have no competing interests.
Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.
Additional file 1: Figure S1. (a) XPS spectrum of Na2Ti3O7 and (b) atomic ratios of elements calculated from XPS spectrum. Figure S2. SEM images of section thicknesses of films (a) F-30, (b) F-45. (c) F-60, (d) F-75. Figure S3. SEM images of modified F-60 film with MTMS aged for 14 h. Figure S4. (a) Nitrogen adsorption-desorption isotherm and (b) pore size distribution of F-60 film. Figure S5. Radical trapping experiments. Figure S6. Contact angle of the membrane after recovery. Figure S7. SEM image of F-60 membrane after the fourth time modified by MTMS.
About this article
Cite this article
Shen, S., Wang, C., Sun, M. et al. Free-Standing Sodium Titanate Ultralong Nanotube Membrane with Oil-Water Separation, Self-Cleaning, and Photocatalysis Properties. Nanoscale Res Lett 15, 22 (2020). https://doi.org/10.1186/s11671-020-3255-9
- Sodium titanate ultralong nanotubes
- Oil-water separation